Eur J Oral Sci 2014; 122: 245–250 DOI: 10.1111/eos.12128 Printed in Singapore. All rights reserved
Ó 2014 The Authors. Eur J Oral Sci published by John Wiley & Sons Ltd
European Journal of Oral Sciences
Simulation of clinical fractures for three different all-ceramic crowns Øilo M, Kvam K, Gjerdet NR. Simulation of clinical fractures for three diﬀerent allceramic crowns. Eur J Oral Sci 2014; 122: 245–250. © 2014 The Authors. Eur J Oral Sci published by John Wiley & Sons Ltd Comparison of fracture strength and fracture modes of diﬀerent all-ceramic crown systems is not straightforward. Established methods for reliable testing of allceramic crowns are not currently available. Published in-vitro tests rarely simulate clinical failure modes and are therefore unsuited to distinguish between the materials. The in-vivo trials usually lack assessment of failure modes. Fractographic analyses show that clinical crowns usually fail from cracks initiating in the cervical margins, whereas in-vitro specimens fail from contact damage at the occlusal loading point. The aim of this study was to compare three all-ceramic systems using a clinically relevant test method that is able to simulate clinical failure modes. Ten incisor crowns of three types of all-ceramic systems were exposed to soft loading until fracture. The initiation and propagation of cracks in these crowns were compared with those of a reference group of crowns that failed during clinical use. All crowns fractured in a manner similar to fracture of the clinical reference crowns. The zirconia crowns fractured at statistically signiﬁcantly higher loads than alumina and glass-ceramic crowns. Fracture initiation was in the core material, cervically in the approximal areas.
Marit Øilo1, Ketil Kvam2, Nils R. Gjerdet1,2 Department of Clinical Dentistry – Biomaterials, Faculty of Medicine and Dentistry, University of Bergen, Bergen; 2 Nordic Institute of Dental Materials, NIOM, Oslo, Norway 1
Marit Øilo, Department of Clinical Dentistry – Biomaterials, Faculty of Medicine and Dentistry, University of Bergen, Postboks 7804, N-5020 Bergen, Norway E-mail: [email protected]
.uib.no Key words: alumina; dental ceramics; fracture; glass-ceramic; zirconia This is an open access article under the terms of the Creative Commons Attribution-NonCommercial-NoDerivs License, which permits use and distribution in any medium, provided the original work is properly cited, the use is non-commercial and no modifications or adaptations are made. The copyright line for this article was changed on 22nd September 2014 after original online publication.
Accepted for publication February 2014
There has been a steady development of stronger and more versatile ceramic materials for dental use in the last decades. Many variables are decisive for the suitability of a crown material, for instance color, translucency, and fracture strength. Strength estimates by laboratory tests indicate that alumina, zirconia, and lithium disilicate glass-ceramics should be able to withstand relevant forces present during oral function for single crowns (1–3). Nevertheless, fractures are one of the main problems reported in clinical follow up for ceramic restorations (4). Several diﬀerent types of fracture may occur during clinical use. Fractures may be cohesive in the veneering ceramic only (chipping) or adhesive between core and veneer (delamination), or bulk fracture of the core itself may occur. The proportion of the diﬀerent types of clinical fracture modes is poorly documented. Comparison of diﬀerent materials is not straightforward as they are used in diﬀerent ways and are rarely compared in larger randomized clinical trials. Chipping and delamination may have several different causes, such as defects in the veneering material, incorrect cooling rates during veneering, a weak chemical bond between the core and the veneer, and traumatic occlusion. Why core fractures occur during clinical function is less obvious. There are currently no established in-vitro methods for testing the fracture strength of all-ceramic crowns. Laboratory tests commonly used to assess the fracture strength of crownshaped specimens tend to produce fractures starting
from the contact damage caused by the loading device (3, 5–7). These types of fractures are not observed in crowns that have fractured during clinical use (8–12). Therefore, it is not certain whether the in-vitro results are applicable for use in clinical decision making (5). In a previous study it was found that soft occlusal loading on alumina-based ceramic crowns attached to abutment models with a low modulus of elasticity and a Poisson’s ratio similar to that of dentin, can simulate clinical fractures for molar crowns (12, 13). The epoxy abutment is compressed during axial loading, which results in a slight bulging of the abutment. The bulging creates tension in the cervical region of the crown ﬁxed to the abutment and fracture occurs at the cervical margin. The load at fracture registered with this method was clinically relevant. It is important to assess this method for diﬀerent types of preparations and diﬀerent types of crown materials in order to evaluate further the method’s general applicability and clinical relevancy (13). The aim of this study was to evaluate the fracture patterns and load at fracture of alumina, zirconia, and glass-ceramic incisor crowns using a newly developed test that induces clinically relevant fractures.
Material and methods Thirty crowns were produced to ﬁt a model of a prepared central incisor (tooth no. 21; Fig. 1). A deep chamfer
Øilo et al.
fracture features were compared with a reference group of 25 crowns (from 21 incisors and four premolars) fractured in clinical use and obtained from Norwegian dentists. Non-parametric statistics were used for the comparison between groups (IBM SPSS statistical software, Armonk, NY, USA). The level of signiﬁcance was set to 0.05.
Results Fig. 1. Specimens as received from the dental technician before veneering. (A) Alumina core, frontal view. (B) Zirconia core, mesial view. (C) Glass-ceramic core, distal view. Note that the glass-ceramic core has thicker walls than both the alumina and zirconia cores.
ﬁnish line was used because this is recommended by most manufacturers of dental ceramics. The model was made as a natural tooth preparation with rounded edges and a ﬁnish line that curved apically on the buccal and palatal surfaces. Ten crowns were made with alumina cores, 10 with zirconia cores, and 10 with glass-ceramic cores (Table 1). The cores of alumina and zirconia were made to a uniform thickness of 0.6 mm. The glass-ceramic cores were built up to an anatomic form that requires only a thin layer of veneering ceramic (Fig. 1). The cores were veneered with veneering ceramics that were suited for the core materials according to the manufacturers’ recommendations. The crowns were luted with zinc phosphate cement (De Trey Zink; Dentsply DeTrey, Konstanz, Germany) to 30 identical epoxy models of the preparation. Excess cement was removed and after a 5-min setting time the crowns were placed in distilled water at 37°C for at least 24 h. The crowns were subsequently loaded at the incisal edge with a ﬂat, steel cylinder of 30 mm in diameter cushioned with a 2-mm-thick rubber disc of hardness 90 Shore A (EPDM 90) to avoid contact damage (Fig. 2). The load was applied in a universal materials testing system at 0.5 mm min 1 until fracture occurred (Lloyd Instruments, Leicester, UK). The procedure was performed with the crowns immersed in water at 37°C. Load at fracture was recorded. The procedure was recorded by video camera for all crowns. The fractured crowns were analyzed using fractographic methods (14). The fracture start of the main, primary fracture was localized for each crown. Secondary fractures and general crack propagation was also mapped. The fracture analysis results were compared with the video recordings to verify the crack start and crack propagation. The
All crowns, except one zirconia crown, fractured through both core and veneer. There were statistically signiﬁcant diﬀerences among the groups (Kruskall– Wallis test P < 0.001, Fig. 3). The fracture loads of the zirconia-based crowns were statistically signiﬁcantly higher than were those of the other two materials (Mann–Whitney U-test P < 0.001). There was no statistically signiﬁcant diﬀerence between the alumina and glass-ceramic crowns (Mann–Whitney U-test P = 0.25). The fracture modes achieved with the test methods resembled the fracture patterns observed in clinical failures of the retrieved reference crowns (Fig. 4). The fracture modes are presented in Fig. 5. All primary core fractures were initiated in the cervical area in the approximal region, as observed in the clinical reference group. One crown with a zirconia core delaminated completely between the core and the buccal veneering ceramic (adhesive fracture). This fracture started on the incisal edge from contact damage. The core of this crown remained intact. A similar fracture was observed in one of the clinical reference crowns with zirconia although this was a cohesive fracture within the veneer. All the other zirconia crowns exhibited partial delamination of the veneering ceramic in addition to the core fractures. No delamination was observed on the other two crown types. Minor secondary chipping of the veneering ceramic was observed in all crowns (cohesive fractures). Twenty-three of the 30 test crowns exhibited secondary fractures in the core material. These were mainly caused by bifurcations of the main fracture (16 specimens) and new cracks starting at the opposite side of the crown margin compared with the start of the primary fracture (seven specimens). These ﬁndings are similar to those of the clinical reference group.
Table 1 Details of the materials used in the trial Material group
Manufacturer Vita Zahnfabrik, Bad S€ackingen, Germany HD, H.C. Stark Ceramics, Selb, Germany Ivoclar Vivadent
Vita In-Ceram AL for inLab
ZrO2 99% (HfO2/Y2O3) Al2O3 0.25% LiSi2O5 70% SiO2 30% (K2O, P2O5, ZrO2, ZnO)
Starceram Z-Al-Med HD
IPS e.max Press
Veneering material Ducera AllCeram, Degudent, Hanau, Germany IPS e-max Ceram, Ivoclar Vivadent, Schaan, Liechtenstein IPS e-max Ceram, Ivoclar Vivadent
Simulation of clinical ceramic fractures
Fig. 2. The test set up. The crowns are cemented to an epoxy model of the tooth preparations. Axial load is applied on the incisal edge at 1 mm min 1 (red arrow), but cushioned to avoid contact damage. The load causes the epoxy model to compress vertically and expand horizontally (blue arrow), which causes tension at the cervical margin of the crown. The area of expected concentration of tension is marked with a red arrow at the top of the curvature.
Fig. 3. Box-plot of the load at fracture in Newton (N) for the three diﬀerent groups. The median values are indicated as horizontal lines in the box, and the bars represent the maximum and minimum values.
Discussion The provoked in-vitro fracture modes closely matched the in-vivo fracture modes observed in retrieved reference crowns, indicating that the test method is well suited for simulating clinical stress in all-ceramic crowns. Vertical tension in the cervical crown margin seems to have initiated fractures from the cervical margin in the approximal area. The tension is diﬃcult to measure but seems to be created by clinically relevant axial loads. The diﬀerences among materials are therefore relevant for clinical application. The ﬁnding that zirconia was stronger than the other two materials is in accordance with previous ﬁndings and assumptions (15–18). However, the mean fracture load was lower than in previous studies of crown-shaped specimens (3, 19–24). This is probably caused by the diﬀerences in crack initiation. In the present study the fractures were initiated in the cervical margin as a result of tension created by the
expanding abutment, as observed in a previous study that used the same method (13). The cervical margin is the thinnest area of the crown and the area most susceptible to machining damage (25). The occlusal surface is usually the thickest area of the crown; furthermore, the occlusal surface is supported by the occlusal area of the tooth. In previous in-vitro trials the fractures have been initiated from occlusal contact damage (5) or from cone cracks under the occlusal surface (10, 26). With a rigid abutment material, the tensile stress at the cervical margin will be lower. Therefore, higher loads are required to obtain fractures. However, few clinical core–veneer crowns have had the same fracture mode as presented in these in-vitro tests. Clinically fractured crowns may have many diﬀerent fracture modes depending on the material, design, and load. Chipping is probably the most common fracture occurring in clinical use. However, it is more complicated to retrieve such fractures without damaging the remaining crown. Bulk fractures or chipping have been shown to start from contact damage on the occlusal surface in monolayer crowns without high-strength cores (26). Furthermore, fractures starting from the inner surface of the core in the occlusal area as a result of radial cracks have been presented both in clinical failures (10, 26, 27) and in laboratory failures (28). The focus of this study was to simulate the fracture modes observed in the retrieved clinical fractures we received and thus the aim was to avoid the other types of fracture modes. To fully comprehend the behavior of allceramic crowns, all clinical failure modes must be investigated further. Clinical trials rarely include thorough analyses of failure modes. So far, it seems that chipping is more predominant than core failures, especially for zirconia crowns (4, 29). Nevertheless, zirconia core failures do occur in spite of the high strength, and it would be of interest to ﬁnd out why. The ﬁnding, in the present study, that all core fractures started in the approximal area indicates that this is the weakest point of the crowns or the area that is most exposed to tension. This may be explained by the diﬀerences in mechanical properties between dentin and dental ceramics. Ceramics are stiﬀ and brittle and deform very little before fracture during loading (30, 31). However, dentin is elastic and will deform during loading (32, 33). A high occlusal load will compress the dentin, resulting in an increase in the diameter of the tooth cervically (bulging), which in turn will cause tension at the crown margins (hoop forces) (Fig. 2). A previous study revealed that an expansion of 0.1% was suﬃcient to cause a fracture of alumina crowns for molars (13). It was not possible to measure reliably the bucco–palatal expansion of the cervical crown margin for the present specimens, but it is reasonable to assume that an expansion of approximately 7 lm has occurred. The crown margins are usually not even or leveled, creating stress foci in the areas that curve toward the occlusal surface (e.g. approximal). This curve is often located where the crown height is lowest, which gives a shorter axial wall. The combination of the curvature and the shorter axial wall in this area is
Øilo et al.
Fig. 4. Fractographic map of a zirconia crown fractured in vitro by simulation of clinical fracture. The boxes indicate size and location of the magniﬁed images surrounding the central image. Dotted arrow indicate crack propagation, Black arrow indicate fracture origin and white arrow indicate fracture end.
Fig. 5. Typical fracture modes in the diﬀerent material categories for the test crowns and the crowns in the reference group. n, number of crowns in each group. The arrows indicate the start of the fracture.
probably the reason that most fractures start here. Finite element analyses have found increased concentration of stress in the cervical margin with increased diﬀerence in axial wall height in the bucco–palatal walls compared with the mesial–distal walls (34). However,
the observed fractures in the test specimen and the reference crowns do not follow the shortest path across to the other side. This indicates that the fracture is not caused only by the shorter wall height. The zirconia crowns displayed delamination of the veneer during fracture, whereas the other two crown types only had minor chipping within the veneering ceramics. These ﬁndings are in accordance with clinical ﬁndings where chipping is reported more frequently for zirconia-based restorations than for other all-ceramic restorations (31, 35–37). Moreover, event though adhesive fractures were found in all zirconia crowns, these occurred at a higher load than the fracture load in the other groups. The crown with total delamination differed signiﬁcantly from all other test crowns, but was similar to an in-vivo crown that had been removed as a result of fracture of veneering ceramic only. This type of delamination fracture is usually called ‘chipping’ in clinical trials. Such a failure would nevertheless have been classiﬁed as a ‘clinical failure’ and would require replacement owing to the large impact on function and esthetics. Chipping damage is more frequently observed in clinical trials and has been successfully simulated in vitro previously. All these ﬁndings indicate that the results are clinically relevant and can be used for clinical decision making. Furthermore, they indicate that the test method is well suited for comparing load at fracture and fracture modes of diﬀerent all-ceramic crowns. The glass-ceramic crowns achieved similar fracturestrength values as the alumina-based crowns, even though glass-ceramic is a weaker material, as measured in ﬂexural strength tests of bar-shaped specimens (15).
Simulation of clinical ceramic fractures
This may be explained by the diﬀerences in the geometry of the cores at the crown margin (Fig. 1). The alumina cores had a uniform thickness of 0.6 mm with a thin edge at the crown margin to allow room for veneering ceramic all the way down to the margin, allowing the opaque, uniform color of the alumina to be covered. The glass-ceramic cores are more translucent than alumina and can be made in many diﬀerent tooth colors. It is not necessary to have veneering material all the way to the margin on these crowns in order to achieve optimal esthetics. These cores were built up to an anatomic form and with a thicker crown edge than on the alumina and zirconia copings. The glass-ceramic cores were covered with thinner layers of veneer and glaze than the alumina and zirconia coping to achieve an anatomically correct crown. When evaluating the fracture strength in this trial it must be taken into consideration that the glass-ceramic crowns can probably achieve better strength values clinically when adhesive luting agents are used (38). The information from the manufacturers indicates that both conventional and adhesive luting agents can be used. However, adhesive cementation is recommended for optimal strength. Several in-vitro studies have been performed to assess the importance of the geometry of the ﬁnish line, but the results of the diﬀerent trials are ambiguous. Some trials ﬁnd that the deeper the chamfer, the stronger the crown; others ﬁnd no signiﬁcant diﬀerence (7, 39–41). As most of these trials have loaded the crowns in such a way that the fractures start occlusally or on the incisal edge, it is not surprising that the eﬀect of the ﬁnish-line design is limited. One study, using a method similar to that of the present study, found that the geometry of the ﬁnish line is of great importance to both fracture initiation and fracture strength for dome-shaped glass structures (11). Further studies, using clinically relevant test methods, must be performed to verify the eﬀect of ﬁnish-line geometry for dental ceramic crowns in order to recommend changes in the design of the restoration or the preparation. The newly developed test method is well suited for assessing the clinically relevant fracture load of diﬀerent all-ceramic crown materials. All the tested crowns fractured at loads that indicate suitability for clinical use in anterior crowns. Acknowledgements – We are grateful for the assistance of the dental technician students Magnus Hakan Iseri and Adriane Andersen Mougios in the design and production of the core structures. Conﬂicts of interest – The authors declare that no conﬂicts of interest exist for any of the products or equipment mentioned in the paper.
References 1. FERRARIO VF, SFORZA C, ZANOTTI G, TARTAGLIA GM. Maximal bite forces in healthy young adults as predicted by surface electromyography. J Dent 2004; 32: 451–457. 2. SENYILMAZ DP, CANAY S, HEYDECKE G, STRUB JR. Inﬂuence of thermomechanical fatigue loading on the fracture resistance of all-ceramic posterior crowns. Eur J Prosthodont Restor Dent 2010; 18: 50–54.
3. CAMPOS RE, SOARES CJ, QUAGLIATTO PS, SOARES PV, DE OLIVEIRA OB Jr, SANTOS-FILHO PC, SALAZAR-MAROCHO SM. In vitro study of fracture load and fracture pattern of ceramic crowns: a ﬁnite element and fractography analysis. J Prosthodont 2011; 20: 447–455. 4. PJETURSSON BE, SAILER I, ZWAHLEN M, HAMMERLE CH. A systematic review of the survival and complication rates of all-ceramic and metal-ceramic reconstructions after an observation period of at least 3 years. Part I: single crowns. Clin Oral Implants Res 2007; 18 (Suppl 3): 73–85. 5. KELLY JR, BENETTI P, RUNGRUANGANUNT P, BONA AD. The slippery slope: critical perspectives on in vitro research methodologies. Dent Mater 2012; 28: 41–51. 6. ANUSAVICE KJ, KAKAR K, FERREE N. Which mechanical and physical testing methods are relevant for predicting the clinical performance of ceramic-based dental prostheses? Clin Oral Implants Res 2007; 18 (Suppl 3): 218–231. 7. ABOUSHELIB MN. Fatigue and fracture resistance of zirconia crowns prepared with diﬀerent ﬁnish line designs. J Prosthodont 2012; 21: 22–27. 8. QUINN JB, QUINN GD, KELLY JR, SCHERRER SS. Fractographic analyses of three ceramic whole crown restoration failures. Dent Mater 2005; 21: 920–929. 9. SCHERRER SS, QUINN GD, QUINN JB. Fractographic failure analysis of a Proceraâ AllCeram crown using stereo and scanning electron microscopy. Dent Mater 2008; 24: 1107– 1113. 10. SCHERRER SS, QUINN JB, QUINN GD, KELLY JR. Failure analysis of ceramic clinical cases using qualitative fractography. Int J Prosthodont 2006; 19: 185–192. 11. WHITTON A, QASIM T, FORD C, HU XZ, BUSH M. The role of skirt geometry of dental crowns on the mechanics of failure: experimental and numerical study. Med Eng Phys 2008; 30: 661–668. 12. ØILO M, GJERDET NR. Fractographic analysis of all-ceramic crowns: a study of 27 clinically-fractured crowns. Dent Mater 2013; 29: e78–e84. 13. ØILO M, KVAM K, TIBBALLS JE, GJERDET NR. Clinically relevant fracture testing of all-ceramic crowns. Dent Mater 2013; 29: 815–823. 14. QUINN GD. Fractography of ceramics and glasses. Washington: National Institute of Standards and Technology, 2007. 15. ØILO M, TVINNEREIM HM, GJERDET NR. Qualitative and quantitative fracture analyses of high-strength ceramics. Eur J Oral Sci 2009; 117: 187–193. 16. GUAZZATO M, ALBAKRY M, RINGER SP, SWAIN MV. Strength, fracture toughness and microstructure of a selection of allceramic materials. Part II. Zirconia-based dental ceramics. Dent Mater 2004; 20: 449–456. 17. GUAZZATO M, ALBAKRY M, RINGER SP, SWAIN MV. Strength, fracture toughness and microstructure of a selection of allceramic materials. Part I. Pressable and alumina glass-inﬁltrated ceramics. Dent Mater 2004; 20: 441–448. 18. STRUB JR, BESCHNIDT SM. Fracture strength of 5 diﬀerent allceramic crown systems. Int J Prosthodont 1998; 11: 602–609. 19. KIM JH, LEE SJ, PARK JS, RYU JJ. Fracture load of monolithic CAD/CAM lithium disilicate ceramic crowns and veneered zirconia crowns as a posterior implant restoration. Implant Dent 2013; 22: 66–70. 20. YUCEL MT, YONDEM I, AYKENT F, ERASLAN O. Inﬂuence of the supporting die structures on the fracture strength of allceramic materials. Clin Oral Invest 2012; 16: 1105–1110. 21. STAWARCZYK B, OZCAN M, HAMMERLE CH, ROOS M. The fracture load and failure types of veneered anterior zirconia crowns: an analysis of normal and Weibull distribution of complete and censored data. Dent Mater 2012; 28: 478–487. 22. LARSSON C, EL MADHOUN S, WENNERBERG A, VULT VON STEYERN P. Fracture strength of yttria-stabilized tetragonal zirconia polycrystals crowns with diﬀerent design: an in vitro study. Clin Oral Implants Res 2012; 23: 820–826. 23. HEINTZE SD, ALBRECHT T, CAVALLERI A, STEINER M. A new method to test the fracture probability of all-ceramic crowns with a dual-axis chewing simulator. Dent Mater 2011; 27: e10–e19.
Øilo et al.
24. REKOW ED, ZHANG G, THOMPSON V, KIM JW, COEHLO P, ZHANG Y. Eﬀects of geometry on fracture initiation and propagation in all-ceramic crowns. J Biomed Mater Res B Appl Biomater 2009; 88: 436–446. 25. DENRY I. How and when does fabrication damage adversely aﬀect the clinical performance of ceramic restorations? Dent Mater 2013; 29: 85–96. 26. KELLY JR, GIORDANO R, POBER R, CIMA MJ. Fracture surface analysis of dental ceramics: clinically failed restorations. Int J Prosthodont 1990; 3: 430–440. 27. THOMPSON JY, ANUSAVICE KJ, NAMAN A, MORRIS HF. Fracture surface characterization of clinically failed all-ceramic crowns. J Dent Res 1994; 73: 1824–1832. 28. KELLY JR, RUNGRUANGANUNT P, HUNTER B, VAILATI F. Development of a clinically validated bulk failure test for ceramic crowns. J Prosthet Dent 2010; 104: 228–238. 29. RAIGRODSKI AJ, HILLSTEAD MB, MENG GK, CHUNG K-H. Survival and complications of zirconia-based ﬁxed dental prostheses: a systematic review. J Prosthet Dent 2012; 107: 170–177. 30. RIZKALLA AS, JONES DW. Mechanical properties of commercial high strength ceramic core materials. Dent Mater 2004; 20: 207–212. 31. DENRY I, KELLY JR. State of the art of zirconia for dental applications. Dent Mater 2008; 24: 299–307. 32. KINNEY JH, MARSHALL SJ, MARSHALL GW. The mechanical properties of human dentin: a critical review and re-evaluation of the dental literature. Crit Rev Oral Biol Med 2003; 14: 13–29. 33. ZAYTSEV D, GRIGORIEV S, PANFILOV P. Deformation behavior of human dentin under uniaxial compression. Int J Biomater 2012; 2012: 854539.
34. COELHO PG, SILVA NR, THOMPSON VP, REKOW D, ZHANG G. Eﬀect of proximal wall height on all-ceramic crown core stress distribution: a ﬁnite element analysis study. Int J Prosthodont 2009; 22: 78–86. 35. MOLIN MK, KARLSSON SL. Five-year clinical prospective evaluation of zirconia-based Denzir 3-unit FPDs. Int J Prosthodont 2008; 21: 223–227. 36. OZKURT Z, KAZAZOGLU E. Clinical success of zirconia in dental applications. J Prosthodont 2009; 19: 64–68. 37. SAILER I, PJETURSSON BE, ZWAHLEN M, HAMMERLE CH. A systematic review of the survival and complication rates of all-ceramic and metal-ceramic reconstructions after an observation period of at least 3 years. Part II: ﬁxed dental prostheses. Clin Oral Implants Res 2007; 18 (Suppl 3): 86–96. € € H, MORMANN WH. Strength and fracture 38. BINDL A, LUTHY pattern of monolithic CAD/CAM-generated posterior crowns. Dent Mater 2006; 22: 29–36. 39. BERNAL G, JONES RM, BROWN DT, MUNOZ CA, GOODACRE CJ. The eﬀect of ﬁnish line form and luting agent on the breaking strength of Dicor crowns. Int J Prosthodont 1993; 6: 286–290. 40. REICH S, PETSCHELT A, LOHBAUER U. The eﬀect of ﬁnish line preparation and layer thickness on the failure load and fractography of ZrO2 copings. J Prosthet Dent 2008; 99: 369– 376. 41. VULT VON STEYERN P, AL-ANSARI A, WHITE K, NILNER K, DERAND T. Fracture strength of In-Ceram all-ceramic bridges in relation to cervical shape and try-in procedure. An in-vitro study. Eur J Prosthodont Restor Dent 2000; 8: 153– 158.